General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.9 - 7.92 g/cm³ Show Material materials with Density of 7.9 - 7.92 g/cm³ |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | -100.0 °C | 206 GPa Show Material materials with Elastic modulus of 206 GPa |

20.0 °C | 196 - 200 GPa Show Material materials with Elastic modulus of 196 - 200 GPa | |

24.0 °C | 194.4 - 196.5 GPa Show Material materials with Elastic modulus of 194.4 - 196.5 GPa | |

100.0 °C | 190 - 194 GPa Show Material materials with Elastic modulus of 190 - 194 GPa | |

149.0 °C | 188.2 - 189.6 GPa Show Material materials with Elastic modulus of 188.2 - 189.6 GPa | |

200.0 °C | 182 - 186 GPa Show Material materials with Elastic modulus of 182 - 186 GPa | |

260.0 °C | 182.7 - 184.1 GPa Show Material materials with Elastic modulus of 182.7 - 184.1 GPa | |

300.0 °C | 174 - 179 GPa Show Material materials with Elastic modulus of 174 - 179 GPa | |

371.0 °C | 173.1 - 177.9 GPa Show Material materials with Elastic modulus of 173.1 - 177.9 GPa | |

400.0 °C | 166 - 172 GPa Show Material materials with Elastic modulus of 166 - 172 GPa | |

483.0 °C | 157.9 - 160 GPa Show Material materials with Elastic modulus of 157.9 - 160 GPa | |

500.0 °C | 158 - 165 GPa Show Material materials with Elastic modulus of 158 - 165 GPa | |

593.0 °C | 149.6 - 155.8 GPa Show Material materials with Elastic modulus of 149.6 - 155.8 GPa | |

600.0 °C | 150 GPa Show Material materials with Elastic modulus of 150 GPa | |

700.0 °C | 142 GPa Show Material materials with Elastic modulus of 142 GPa | |

704.0 °C | 137.9 - 144.8 GPa Show Material materials with Elastic modulus of 137.9 - 144.8 GPa | |

800.0 °C | 134 GPa Show Material materials with Elastic modulus of 134 GPa | |

816.0 °C | 120.7 - 128.2 GPa Show Material materials with Elastic modulus of 120.7 - 128.2 GPa | |

Elongation | 20.0 °C | 45 % Show Material materials with Elongation of 45 % |

Poisson's ratio | 20.0 °C | 0.28 [-] Show Material materials with Poisson's ratio of 0.28 [-] |

24.0 °C | 0.24 - 0.25 [-] Show Material materials with Poisson's ratio of 0.24 - 0.25 [-] | |

149.0 °C | 0.27 - 0.3 [-] Show Material materials with Poisson's ratio of 0.27 - 0.3 [-] | |

260.0 °C | 0.29 - 0.32 [-] Show Material materials with Poisson's ratio of 0.29 - 0.32 [-] | |

371.0 °C | 0.32 [-] Show Material materials with Poisson's ratio of 0.32 [-] | |

483.0 °C | 0.27 - 0.29 [-] Show Material materials with Poisson's ratio of 0.27 - 0.29 [-] | |

593.0 °C | 0.29 - 0.3 [-] Show Material materials with Poisson's ratio of 0.29 - 0.3 [-] | |

704.0 °C | 0.27 - 0.3 [-] Show Material materials with Poisson's ratio of 0.27 - 0.3 [-] | |

816.0 °C | 0.23 - 0.27 [-] Show Material materials with Poisson's ratio of 0.23 - 0.27 [-] | |

Unlock all property charts | ||

Shear modulus | 24.0 °C | 78.6 GPa Show Material materials with Shear modulus of 78.6 GPa |

149.0 °C | 72.4 - 74.5 GPa Show Material materials with Shear modulus of 72.4 - 74.5 GPa | |

260.0 °C | 69.6 - 71 GPa Show Material materials with Shear modulus of 69.6 - 71 GPa | |

371.0 °C | 65.5 - 67.6 GPa Show Material materials with Shear modulus of 65.5 - 67.6 GPa | |

483.0 °C | 62.1 GPa Show Material materials with Shear modulus of 62.1 GPa | |

593.0 °C | 57.9 - 60 GPa Show Material materials with Shear modulus of 57.9 - 60 GPa | |

704.0 °C | 54.5 - 55.9 GPa Show Material materials with Shear modulus of 54.5 - 55.9 GPa | |

816.0 °C | 49 - 50.3 GPa Show Material materials with Shear modulus of 49 - 50.3 GPa | |

Unlock all property charts | ||

Tensile strength | 20.0 °C | 500 - 700 MPa Show Material materials with Tensile strength of 500 - 700 MPa |

50.0 °C | 480 MPa Show Material materials with Tensile strength of 480 MPa | |

100.0 °C | 450 MPa Show Material materials with Tensile strength of 450 MPa | |

150.0 °C | 420 MPa Show Material materials with Tensile strength of 420 MPa | |

200.0 °C | 400 MPa Show Material materials with Tensile strength of 400 MPa | |

250.0 °C | 390 MPa Show Material materials with Tensile strength of 390 MPa | |

300.0 °C | 380 MPa Show Material materials with Tensile strength of 380 MPa | |

350.0 °C | 380 MPa Show Material materials with Tensile strength of 380 MPa | |

400.0 °C | 380 MPa Show Material materials with Tensile strength of 380 MPa | |

450.0 °C | 375 MPa Show Material materials with Tensile strength of 375 MPa | |

500.0 °C | 360 MPa Show Material materials with Tensile strength of 360 MPa | |

550.0 °C | 335 MPa Show Material materials with Tensile strength of 335 MPa | |

600.0 °C | 300 MPa Show Material materials with Tensile strength of 300 MPa | |

Unlock all property charts | ||

Yield strength Rp0.2 | 20.0 °C | 190 MPa Show Material materials with Yield strength Rp0.2 of 190 MPa |

50.0 °C | 177 MPa Show Material materials with Yield strength Rp0.2 of 177 MPa | |

100.0 °C | 155 MPa Show Material materials with Yield strength Rp0.2 of 155 MPa | |

150.0 °C | 140 MPa Show Material materials with Yield strength Rp0.2 of 140 MPa | |

200.0 °C | 127 MPa Show Material materials with Yield strength Rp0.2 of 127 MPa | |

250.0 °C | 118 MPa Show Material materials with Yield strength Rp0.2 of 118 MPa | |

300.0 °C | 110 MPa Show Material materials with Yield strength Rp0.2 of 110 MPa | |

350.0 °C | 104 MPa Show Material materials with Yield strength Rp0.2 of 104 MPa | |

400.0 °C | 98 MPa Show Material materials with Yield strength Rp0.2 of 98 MPa | |

450.0 °C | 95 MPa Show Material materials with Yield strength Rp0.2 of 95 MPa | |

500.0 °C | 92 MPa Show Material materials with Yield strength Rp0.2 of 92 MPa | |

550.0 °C | 90 MPa Show Material materials with Yield strength Rp0.2 of 90 MPa | |

Unlock all property charts |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.49E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.49E-5 1/K | |

20.0 °C | 1.61E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.61E-5 1/K | ||

100.0 °C | 1.6E-5 - 1.67E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.6E-5 - 1.67E-5 1/K | ||

200.0 °C | 1.65E-5 - 1.72E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.65E-5 - 1.72E-5 1/K | ||

300.0 °C | 1.7E-5 - 1.77E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.7E-5 - 1.77E-5 1/K | ||

400.0 °C | 1.75E-5 - 1.81E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.75E-5 - 1.81E-5 1/K | ||

500.0 °C | 1.8E-5 - 1.84E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.8E-5 - 1.84E-5 1/K | ||

600.0 °C | 1.88E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.88E-5 1/K | ||

700.0 °C | 1.91E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.91E-5 1/K | ||

800.0 °C | 1.94E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.94E-5 1/K | ||

Unlock all property charts | |||

Max service temperature, long | -200 - 550 °C Show Material materials with Max service temperature, long of -200 - 550 °C | ||

Melting point | 1230 - 1480 °C Show Material materials with Melting point of 1230 - 1480 °C | Typical for Austenitic Stainless Steel | |

Specific heat capacity | -100.0 °C | 440 J/(kg·K) Show Material materials with Specific heat capacity of 440 J/(kg·K) | |

20.0 °C | 472 - 500 J/(kg·K) Show Material materials with Specific heat capacity of 472 - 500 J/(kg·K) | ||

100.0 °C | 487 J/(kg·K) Show Material materials with Specific heat capacity of 487 J/(kg·K) | ||

200.0 °C | 503 J/(kg·K) Show Material materials with Specific heat capacity of 503 J/(kg·K) | ||

300.0 °C | 512 J/(kg·K) Show Material materials with Specific heat capacity of 512 J/(kg·K) | ||

400.0 °C | 520 J/(kg·K) Show Material materials with Specific heat capacity of 520 J/(kg·K) | ||

500.0 °C | 530 J/(kg·K) Show Material materials with Specific heat capacity of 530 J/(kg·K) | ||

600.0 °C | 541 J/(kg·K) Show Material materials with Specific heat capacity of 541 J/(kg·K) | ||

700.0 °C | 551 J/(kg·K) Show Material materials with Specific heat capacity of 551 J/(kg·K) | ||

800.0 °C | 559 J/(kg·K) Show Material materials with Specific heat capacity of 559 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | -100.0 °C | 11.7 W/(m·K) Show Material materials with Thermal conductivity of 11.7 W/(m·K) | |

20.0 °C | 14.5 - 15 W/(m·K) Show Material materials with Thermal conductivity of 14.5 - 15 W/(m·K) | ||

100.0 °C | 16 W/(m·K) Show Material materials with Thermal conductivity of 16 W/(m·K) | ||

200.0 °C | 17.6 W/(m·K) Show Material materials with Thermal conductivity of 17.6 W/(m·K) | ||

300.0 °C | 19.1 W/(m·K) Show Material materials with Thermal conductivity of 19.1 W/(m·K) | ||

400.0 °C | 20.4 W/(m·K) Show Material materials with Thermal conductivity of 20.4 W/(m·K) | ||

500.0 °C | 21.9 W/(m·K) Show Material materials with Thermal conductivity of 21.9 W/(m·K) | ||

600.0 °C | 23.3 W/(m·K) Show Material materials with Thermal conductivity of 23.3 W/(m·K) | ||

700.0 °C | 24.7 W/(m·K) Show Material materials with Thermal conductivity of 24.7 W/(m·K) | ||

800.0 °C | 26.1 W/(m·K) Show Material materials with Thermal conductivity of 26.1 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | -100.0 °C | 3.7 mm²/s Show Material materials with Thermal diffusivity of 3.7 mm²/s | |

20.0 °C | 3.9 mm²/s Show Material materials with Thermal diffusivity of 3.9 mm²/s | ||

100.0 °C | 4.3 mm²/s Show Material materials with Thermal diffusivity of 4.3 mm²/s | ||

200.0 °C | 4.3 mm²/s Show Material materials with Thermal diffusivity of 4.3 mm²/s | ||

300.0 °C | 4.6 mm²/s Show Material materials with Thermal diffusivity of 4.6 mm²/s | ||

400.0 °C | 4.7 mm²/s Show Material materials with Thermal diffusivity of 4.7 mm²/s | ||

500.0 °C | 4.9 mm²/s Show Material materials with Thermal diffusivity of 4.9 mm²/s | ||

600.0 °C | 5 mm²/s Show Material materials with Thermal diffusivity of 5 mm²/s | ||

700.0 °C | 5.3 mm²/s Show Material materials with Thermal diffusivity of 5.3 mm²/s | ||

800.0 °C | 5.7 mm²/s Show Material materials with Thermal diffusivity of 5.7 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | -100.0 °C | 5.86E-7 Ω·m Show Material materials with Electrical resistivity of 5.86E-7 Ω·m |

20.0 °C | 6.92E-7 - 7.3E-7 Ω·m Show Material materials with Electrical resistivity of 6.92E-7 - 7.3E-7 Ω·m | |

100.0 °C | 7.58E-7 Ω·m Show Material materials with Electrical resistivity of 7.58E-7 Ω·m | |

200.0 °C | 8.36E-7 Ω·m Show Material materials with Electrical resistivity of 8.36E-7 Ω·m | |

300.0 °C | 9.07E-7 Ω·m Show Material materials with Electrical resistivity of 9.07E-7 Ω·m | |

400.0 °C | 9.73E-7 Ω·m Show Material materials with Electrical resistivity of 9.73E-7 Ω·m | |

500.0 °C | 1.02E-6 Ω·m Show Material materials with Electrical resistivity of 1.02E-6 Ω·m | |

600.0 °C | 1.06E-6 Ω·m Show Material materials with Electrical resistivity of 1.06E-6 Ω·m | |

700.0 °C | 1.1E-6 Ω·m Show Material materials with Electrical resistivity of 1.1E-6 Ω·m | |

800.0 °C | 1.13E-6 Ω·m Show Material materials with Electrical resistivity of 1.13E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.07 % Show Material materials with Carbon of 0.07 % |

Chromium | 17 - 19.5 % Show Material materials with Chromium of 17 - 19.5 % |

Manganese | 2 % Show Material materials with Manganese of 2 % |

Nickel | 8 - 10.5 % Show Material materials with Nickel of 8 - 10.5 % |

Nitrogen | 0.1 % Show Material materials with Nitrogen of 0.1 % |

Phosphorus | 0.05 % Show Material materials with Phosphorus of 0.05 % |

Silicon | 1 % Show Material materials with Silicon of 1 % |

Sulfur | 0.015 - 0.03 % Show Material materials with Sulfur of 0.015 - 0.03 % |